#------------------------------------------------------------------------------
#$Date: 2019-11-17 14:32:33 +0100 (dom 17 de nov de 2019) $
#$Revision: 230902 $
#$URL: svn://www.crystallography.net/cod/cif/7/23/14/7231412.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_7231412
loop_
_publ_author_name
'Collings, Ines E.'
'Manna, Rudra Sekhar'
'Tsirlin, Alexander A.'
'Bykov, Maxim'
'Bykova, Elena'
'Hanfland, Michael'
'Gegenwart, Philipp'
'van Smaalen, Sander'
'Dubrovinsky, Leonid'
'Dubrovinskaia, Natalia'
_publ_section_title
;
 Pressure dependence of spin canting in ammonium metal formate
 antiferromagnets.
;
_journal_issue                   37
_journal_name_full               'Physical chemistry chemical physics : PCCP'
_journal_page_first              24465
_journal_page_last               24476
_journal_paper_doi               10.1039/c8cp03761b
_journal_volume                  20
_journal_year                    2018
_chemical_formula_moiety         'C3 H3 Mn O6, N H4'
_chemical_formula_sum            'C3 H7 Mn N O6'
_chemical_formula_weight         208
_space_group_IT_number           4
_space_group_name_Hall           'P 2yb'
_space_group_name_H-M_alt        'P 1 21 1'
_symmetry_cell_setting           monoclinic
_symmetry_Int_Tables_number      4
_symmetry_space_group_name_Hall  'P 2yb'
_symmetry_space_group_name_H-M   'P 1 21 1'
_audit_creation_method           'Jana2006 Version : 25/10/2015'
_audit_update_record
;
2018-08-09 deposited with the CCDC.
2018-08-22 downloaded from the CCDC.
;
_cell_angle_alpha                90
_cell_angle_beta                 116.09(4)
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   6.537(2)
_cell_length_b                   8.4865(16)
_cell_length_c                   7.405(3)
_cell_measurement_reflns_used    239
_cell_measurement_temperature    293
_cell_measurement_theta_max      14.68
_cell_measurement_theta_min      2.01
_cell_volume                     368.9(2)
_computing_cell_refinement       'CrysAlisPro 1.171.38.46 (Rigaku OD, 2015)'
_computing_data_collection       'CrysAlisPro 1.171.38.46 (Rigaku OD, 2015)'
_computing_data_reduction        'CrysAlisPro 1.171.38.46 (Rigaku OD, 2015)'
_diffrn_ambient_pressure         '0.85 GPa'
_diffrn_ambient_temperature      293
_diffrn_detector                 'CCD plate'
_diffrn_measured_fraction_theta_full 0.96
_diffrn_measured_fraction_theta_max 0.93
_diffrn_measurement_device       'ID15B beamline, ESRF'
_diffrn_measurement_device_type
'esperanto-CrysAlisPro-abstract goniometer imported esperanto images'
_diffrn_measurement_method       'ω scans'
_diffrn_measurement_specimen_support 'diamond-anvil cell'
_diffrn_radiation_monochromator  synchrotron
_diffrn_radiation_probe          x-ray
_diffrn_radiation_source         synchrotron
_diffrn_radiation_type           synchrotron
_diffrn_radiation_wavelength     0.41111
_diffrn_reflns_av_R_equivalents  0.0249
_diffrn_reflns_av_unetI/netI     0.0411
_diffrn_reflns_limit_h_max       8
_diffrn_reflns_limit_h_min       -8
_diffrn_reflns_limit_k_max       9
_diffrn_reflns_limit_k_min       -9
_diffrn_reflns_limit_l_max       9
_diffrn_reflns_limit_l_min       -9
_diffrn_reflns_number            3805
_diffrn_reflns_theta_full        7.18
_diffrn_reflns_theta_max         14.87
_diffrn_reflns_theta_min         1.77
_diffrn_source                   synchrotron
_exptl_absorpt_coefficient_mu    0.379
_exptl_absorpt_correction_T_max  1
_exptl_absorpt_correction_T_min  0.318
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details
;
CrysAlisPro 1.171.38.46 (Rigaku Oxford Diffraction, 2015)
Empirical absorption correction using spherical harmonics,
 implemented in SCALE3 ABSPACK scaling algorithm.
;
_exptl_crystal_colour            colourless
_exptl_crystal_density_diffrn    1.8726
_exptl_crystal_description       block
_exptl_crystal_F_000             202
_exptl_crystal_size_max          0.130
_exptl_crystal_size_mid          0.110
_exptl_crystal_size_min          0.050
_refine_ls_abs_structure_details
'  995 of Friedel pairs used in the refinement'
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_gt    3.14
_refine_ls_goodness_of_fit_ref   2.87
_refine_ls_hydrogen_treatment    constr
_refine_ls_number_constraints    13
_refine_ls_number_parameters     104
_refine_ls_number_reflns         3805
_refine_ls_number_restraints     0
_refine_ls_R_factor_all          0.0876
_refine_ls_R_factor_gt           0.0754
_refine_ls_shift/su_max          0.0356
_refine_ls_shift/su_mean         0.0071
_refine_ls_structure_factor_coef F
_refine_ls_weighting_details     w=1/(σ²(F)+0.0001F²)
_refine_ls_weighting_scheme      sigma
_refine_ls_wR_factor_gt          0.0923
_refine_ls_wR_factor_ref         0.0950
_reflns_number_gt                3016
_reflns_number_total             3805
_reflns_threshold_expression     I>3σ(I)
_cod_data_source_file            c8cp03761b2.cif
_cod_data_source_block           AMnF_c1_p07
_cod_depositor_comments
;
The following automatic conversions were performed:

'_diffrn_radiation_probe' value 'X-ray' changed to 'x-ray' according
to
/home/data/users/saulius/crontab/automatic-downloads/rss-feeds/RSC/lib/dictionaries/cif_core.dic
dictionary named 'cif_core.dic' version 2.4.2 from 2011-04-26.

Automatic conversion script
Id: cif_fix_values 4973 2017-02-22 13:04:09Z antanas 

 Adding full bibliography for 7231402--7231432.cif.
;
_cod_original_formula_sum        'C3 H7 Mn1 N1 O6'
_cod_database_code               7231412
loop_
_space_group_symop_id
_space_group_symop_operation_xyz
1 x,y,z
2 -x,y+1/2,-z
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_adp_type
_atom_site_U_iso_or_equiv
_atom_site_site_symmetry_multiplicity
_atom_site_occupancy
_atom_site_calc_flag
Mn1 Mn 0.66261(17) 0.25 0.32416(12) Uani 0.0424(4) 2 1 d
O1 O 0.8754(9) 0.0990(7) 0.5688(7) Uani 0.059(3) 2 1 d
O2 O 0.3658(9) 0.1170(7) 0.2940(7) Uani 0.054(2) 2 1 d
O3 O 0.7008(10) 0.1003(8) 0.1035(7) Uani 0.060(3) 2 1 d
O4 O 0.9290(9) 0.3819(7) 0.2930(7) Uani 0.057(3) 2 1 d
O5 O 0.6891(9) 0.3982(7) 0.5706(7) Uani 0.058(3) 2 1 d
O6 O 0.4061(8) 0.3994(7) 0.1049(7) Uani 0.054(2) 2 1 d
C1 C 0.9291(13) -0.0402(10) 0.5648(11) Uani 0.058(4) 2 1 d
C2 C 0.3658(14) 0.0378(11) 0.4360(12) Uani 0.065(5) 2 1 d
C3 C 0.4405(14) 0.5003(11) 0.0021(13) Uani 0.056(4) 2 1 d
N1 N -0.0250(9) 0.2519(12) -0.0553(7) Uani 0.054(3) 2 1 d
H1c1 H 0.853233 -0.093935 0.438356 Uiso 0.0698 2 1 d
H1c2 H 0.413245 0.090701 0.562685 Uiso 0.0776 2 1 d
H1c3 H 0.587967 0.502041 0.003476 Uiso 0.067 2 1 d
loop_
_atom_type_symbol
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C -0.0001 0.0005 'International Tables Vol C tables 4.2.6.8 and 6.1.1.1'
H 0.0000 0.0000 'International Tables Vol C tables 4.2.6.8 and 6.1.1.1'
Mn 0.1790 0.2615 'International Tables Vol C tables 4.2.6.8 and 6.1.1.1'
N 0.0006 0.0010 'International Tables Vol C tables 4.2.6.8 and 6.1.1.1'
O 0.0018 0.0018 'International Tables Vol C tables 4.2.6.8 and 6.1.1.1'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle
O1 Mn1 O2 . . 89.7(2)
O1 Mn1 O3 . . 92.2(2)
O1 Mn1 O4 . . 98.3(2)
O1 Mn1 O5 . . 81.6(2)
O1 Mn1 O6 . . 169.2(3)
O2 Mn1 O3 . . 90.7(2)
O2 Mn1 O4 . . 169.20(18)
O2 Mn1 O5 . . 97.2(2)
O2 Mn1 O6 . . 82.2(2)
O3 Mn1 O4 . . 81.9(2)
O3 Mn1 O5 . . 169.9(2)
O3 Mn1 O6 . . 94.9(2)
O4 Mn1 O5 . . 91.1(2)
O4 Mn1 O6 . . 90.6(2)
O5 Mn1 O6 . . 92.3(2)
Mn1 O1 C1 . . 129.3(5)
Mn1 O2 C2 . . 121.6(4)
Mn1 O3 C3 . 2_645 125.0(7)
Mn1 O4 C1 . 2_756 121.3(6)
Mn1 O5 C2 . 2_656 127.8(5)
Mn1 O6 C3 . . 125.6(5)
O1 C1 O4 . 2_746 127.0(7)
O1 C1 H1c1 . . 116.52
O4 C1 H1c1 2_746 . 116.52
O2 C2 O5 . 2_646 126.3(8)
O2 C2 H1c2 . . 116.86
O5 C2 H1c2 2_646 . 116.86
O3 C3 O6 2_655 . 125.2(9)
O3 C3 H1c3 2_655 . 117.39
O6 C3 H1c3 . . 117.39
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_site_symmetry_2
_geom_bond_distance
Mn1 O1 . 2.154(5)
Mn1 O2 . 2.170(6)
Mn1 O3 . 2.169(7)
Mn1 O4 . 2.166(7)
Mn1 O5 . 2.160(6)
Mn1 O6 . 2.159(5)
O1 C1 . 1.237(11)
O2 C2 . 1.248(11)
O3 C3 2_645 1.245(10)
O4 C1 2_756 1.244(9)
O5 C2 2_656 1.233(11)
O6 C3 . 1.230(12)
C1 H1c1 . 0.96
C2 H1c2 . 0.96
C3 H1c3 . 0.96
loop_
_twin_individual_id
_twin_individual_mass_fraction_refined
_twin_individual_twin_matrix_11
_twin_individual_twin_matrix_12
_twin_individual_twin_matrix_13
_twin_individual_twin_matrix_21
_twin_individual_twin_matrix_22
_twin_individual_twin_matrix_23
_twin_individual_twin_matrix_31
_twin_individual_twin_matrix_32
_twin_individual_twin_matrix_33
1 0.242(3) 1 0 0 0 1 0 0 0 1
2 0.1450(13) 1 0 0 0 -1 0 0.7765 0 -1
3 0.1133(11) -0.0759 0 -1.0923 0 1 0 0.8512 0 -0.9241
4 0.1000(11) -0.9241 0 1.0923 0 -1 0 0.1336 0 0.9241
5 0.1595(11) -0.9241 0 1.0923 0 1 0 -0.8512 0 -0.0759
6 0.2405(16) -0.0759 0 -1.0923 0 -1 0 -0.9101 0 0.0759
